- 152 Views
- Uploaded on
- Presentation posted in: General

CHAPTER 5: DIFFUSION IN SOLIDS

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

ISSUES TO ADDRESS...

• How does diffusion occur?

• Why is it an important part of processing?

• How can the rate of diffusion be predicted for

some simple cases?

• How does diffusion depend on structure

and temperature?

1

• Glass tube filled with water.

• At time t = 0, add some drops of ink to one end

of the tube.

• Measure the diffusion distance, x, over some time.

• Compare the results with theory.

2

• Interdiffusion: In an alloy, atoms tend to migrate

from regions of large concentration.

Initially

After some time

Adapted from Figs. 5.1 and 5.2, Callister 6e.

3

• Self-diffusion: In an elemental solid, atoms

also migrate.

Label some atoms

After some time

4

Substitutional Diffusion:

• applies to substitutional impurities

• atoms exchange with vacancies

• rate depends on:

--number of vacancies

--activation energy to exchange.

5

• Simulation of

interdiffusion

across an interface:

• Rate of substitutional

diffusion depends on:

--vacancy concentration

--frequency of jumping.

(Courtesy P.M. Anderson)

6

• Applies to interstitial

impurities.

• More rapid than

vacancy diffusion.

• Simulation:

--shows the jumping of a

smaller atom (gray) from

one interstitial site to

another in a BCC

structure. The

interstitial sites

considered here are

at midpoints along the

unit cell edges.

(Courtesy P.M. Anderson)

7

• Case Hardening:

--Diffuse carbon atoms

into the host iron atoms

at the surface.

--Example of interstitial

diffusion is a case

hardened gear.

Fig. 5.0, Callister 6e.

(Fig. 5.0 is

courtesy of

Surface Division, Midland-Ross.)

• Result: The "Case" is

--hard to deform: C atoms

"lock" planes from shearing.

--hard to crack: C atoms put

the surface in compression.

8

• Doping Silicon with P for n-type semiconductors:

• Process:

1. Deposit P rich

layers on surface.

Fig. 18.0, Callister 6e.

2. Heat it.

3. Result: Doped

semiconductor

regions.

9

• Flux:

• Directional Quantity

• Flux can be measured for:

--vacancies

--host (A) atoms

--impurity (B) atoms

10

• Concentration Profile, C(x): [kg/m3]

Adapted from Fig. 5.2(c), Callister 6e.

• Fick's First Law:

• The steeper the concentration profile,

the greater the flux!

11

• Steady State: the concentration profile doesn't

change with time.

• Apply Fick's First Law:

• If Jx)left = Jx)right , then

• Result: the slope, dC/dx, must be constant

(i.e., slope doesn't vary with position)!

12

• Steel plate at

700C with

geometry

shown:

Adapted from Fig. 5.4, Callister 6e.

• Q: How much

carbon transfers

from the rich to

the deficient side?

13

• Concentration profile,

C(x), changes

w/ time.

• To conserve matter:

• Fick's First Law:

• Governing Eqn.:

14

• Copper diffuses into a bar of aluminum.

Adapted from Fig. 5.5, Callister 6e.

• General solution:

"error function"

Values calibrated in Table 5.1, Callister 6e.

15

• Copper diffuses into a bar of aluminum.

• 10 hours at 600C gives desired C(x).

• How many hours would it take to get the same C(x)

if we processed at 500C?

Key point 1: C(x,t500C) = C(x,t600C).

Key point 2: Both cases have the same Co and Cs.

• Result: Dt should be held constant.

Note: values

of D are

provided here.

• Answer:

16

• The experiment: we recorded combinations of

t and x that kept C constant.

= (constant here)

• Diffusion depth given by:

17

• Experimental result: x ~ t0.58

• Theory predicts x ~ t0.50

• Reasonable agreement!

18

• Diffusivity increases with T.

• Experimental Data:

D has exp. dependence on T

Recall: Vacancy does also!

Adapted from Fig. 5.7, Callister 6e. (Date for Fig. 5.7 taken from E.A. Brandes and G.B. Brook (Ed.) Smithells Metals Reference Book, 7th ed., Butterworth-Heinemann, Oxford, 1992.)

19

Diffusion FASTER for...

• open crystal structures

• lower melting T materials

• materials w/secondary

bonding

• smaller diffusing atoms

• cations

• lower density materials

Diffusion SLOWER for...

• close-packed structures

• higher melting T materials

• materials w/covalent

bonding

• larger diffusing atoms

• anions

• higher density materials

20

Reading: Chapter 5

Homework:

0